Isomeric Sc<sub>2</sub>O@C<sub>78</sub> Related by a Single-Step Stone-Wales Transformation: Key Links in an Unprecedented Fullerene Formation Pathway.
Hao, Yajuan; Tang, Qiangqiang; Li, Xiaohong; Zhang, Meirong; Wan, Yingbo; Feng, Lai; Chen, Ning; Slanina, Zdeněk; Adamowicz, Ludwik; Uhlík, Filip; Inorganic chemistry 55 (2016) 11354–11361; doi:10.1021/acs.inorgchem.6b01894

data_4349077
_publ_section_title
;
 Isomeric Sc<sub>2</sub>O@C<sub>78</sub> Related by a Single-Step
 Stone-Wales Transformation: Key Links in an Unprecedented Fullerene
 Formation Pathway.
;
_journal_issue                   21
_journal_name_full               'Inorganic chemistry'
_journal_page_first              11354
_journal_page_last               11361
_journal_paper_doi               10.1021/acs.inorgchem.6b01894
_journal_volume                  55
_journal_year                    2016
_chemical_formula_moiety         'Sc2O C76, Ni N4 C36 H44, 0.95(bz), 0.05(CF)'
_chemical_formula_sum            'C119.75 H49.75 Cl0.25 N4 Ni O Sc2'
_chemical_formula_weight         1717.88
_chemical_name_common            Sc2O@C78/NiOEP/0.95(bz)0.05(CF)
_space_group_crystal_system      monoclinic
_space_group_IT_number           12
_space_group_name_Hall           '-C 2y'
_space_group_name_H-M_alt        'C 1 2/m 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-2013
_cell_angle_alpha                90
_cell_angle_beta                 92.3050(10)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   25.2588(8)
_cell_length_b                   14.9157(5)
_cell_length_c                   19.5163(6)
_cell_measurement_reflns_used    9989
_cell_measurement_temperature    90(2)
_cell_measurement_theta_max      27.92
_cell_measurement_theta_min      2.73
_cell_volume                     7346.9(4)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-2013 (Sheldrick, 2013)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      90(2)
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.977
_diffrn_measurement_device_type  'Bruker Smart Apex CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1374
_diffrn_reflns_av_unetI/netI     0.1004
_diffrn_reflns_Laue_measured_fraction_full 0.997
_diffrn_reflns_Laue_measured_fraction_max 0.977
_diffrn_reflns_limit_h_max       33
_diffrn_reflns_limit_h_min       -33
_diffrn_reflns_limit_k_max       19
_diffrn_reflns_limit_k_min       -19
_diffrn_reflns_limit_l_max       26
_diffrn_reflns_limit_l_min       -26
_diffrn_reflns_number            65616
_diffrn_reflns_point_group_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.977
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         28.682
_diffrn_reflns_theta_min         2.731
_diffrn_source                   'fine-focus sealed tube'
_exptl_absorpt_coefficient_mu    0.511
_exptl_absorpt_correction_T_max  0.9507
_exptl_absorpt_correction_T_min  0.9273
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS (Sheldrick 1996)'
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    1.553
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             3514
_exptl_crystal_size_max          0.150
_exptl_crystal_size_mid          0.120
_exptl_crystal_size_min          0.100
_platon_squeeze_details
;
;
_refine_diff_density_max         1.127
_refine_diff_density_min         -0.636
_refine_diff_density_rms         0.101
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.085
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     1000
_refine_ls_number_reflns         9605
_refine_ls_number_restraints     1279
_refine_ls_restrained_S_all      1.049
_refine_ls_R_factor_all          0.1430
_refine_ls_R_factor_gt           0.0905
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
;
 w=1/[\s^2^(Fo^2^)+(0.1119P)^2^]
 where P=(Fo^2^+2Fc^2^)/3
;
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1912
_refine_ls_wR_factor_ref         0.2173
_reflns_Friedel_coverage         0.000
_reflns_number_gt                6038
_reflns_number_total             9605
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            ic6b01894_si_002.cif
_cod_data_source_block           shelx
_cod_original_sg_symbol_H-M      'C 2/m'
_cod_database_code               4349077
_shelx_estimated_absorpt_t_min   0.927
_shelx_estimated_absorpt_t_max   0.951
_iucr_refine_squeeze_details
;
TITL Sc2OC78 in C2/m
CELL   25.2590   14.9160   19.5160     90.00     92.31     90.00
SPGR C2/m
C101 0.943 0.139 0.496 !       4.16 eA-3
C102 0.963 0.140 0.546 !       3.97 eA-3
C103 0.508 0.375 0.406 !       3.30 eA-3
C104 0.524 0.368 0.567 !       2.95 eA-3
C105 1.000 0.094 0.502 !       1.83 eA-3
Q106 0.476 0.015 0.126 !       1.72 eA-3
Q107 0.483 0.032 0.045 !       1.63 eA-3
Q108 0.267 0.490 0.657 !       1.10 eA-3
Q109 0.735 0.495 0.422 !       1.08 eA-3
Q110 0.188 0.377 0.737 !       0.98 eA-3
Q111 0.991 0.506 0.907 !       0.91 eA-3
Q112 0.367 0.503 0.266 !       0.88 eA-3
Q113 0.257 0.012 0.439 !       0.86 eA-3
Q114 0.063 0.497 0.015 !       0.84 eA-3
Q115 0.329 0.071 0.313 !       0.84 eA-3
Q116 0.773 0.503 0.312 !       0.82 eA-3
Q117 0.735 0.456 0.703 !       0.81 eA-3
Q118 0.094 0.497 0.235 !       0.78 eA-3
C119 0.992 0.159 0.467 !       0.78 eA-3
Q120 0.949 0.501 0.078 !       0.77 eA-3
Q121 0.495 0.345 0.815 !       0.77 eA-3
Q122 0.304 0.496 0.297 !       0.77 eA-3
Q123 0.789 0.470 0.282 !       0.74 eA-3
Q124 0.664 0.500 0.734 !       0.73 eA-3
Q125 0.259 0.502 0.484 !       0.72 eA-3
Q126 0.717 0.496 0.735 !       0.72 eA-3
Q127 0.554 0.236 0.950 !       0.70 eA-3
Q128 0.837 0.452 0.019 !       0.70 eA-3
Q129 0.947 0.505 0.641 !       0.70 eA-3
Q130 0.094 0.496 0.265 !       0.70 eA-3
Q131 0.844 0.497 0.969 !       0.69 eA-3
Q132 0.695 0.506 0.749 !       0.69 eA-3
Q133 0.008 0.495 0.157 !       0.68 eA-3
Q134 0.763 0.251 0.672 !       0.68 eA-3
Q135 0.742 0.498 0.562 !       0.67 eA-3
Q136 0.358 0.080 0.252 !       0.66 eA-3
Q137 0.328 0.278 0.232 !       0.66 eA-3
Q138 0.290 0.138 0.949 !       0.66 eA-3
Q139 0.704 1.000 0.640 !       0.65 eA-3
Q140 0.204 0.500 0.640 !       0.65 eA-3
Q141 0.499 0.309 0.882 !       0.64 eA-3
Q142 0.680 0.498 0.172 !       0.64 eA-3
Q143 0.758 0.159 0.090 !       0.64 eA-3
Q144 0.211 0.498 0.594 !       0.64 eA-3
Q145 0.088 0.360 0.596 !       0.64 eA-3
Q146 0.744 0.230 0.363 !       0.64 eA-3
Q147 0.538 0.027 0.002 !       0.63 eA-3
Q148 0.064 0.493 0.968 !       0.63 eA-3
Q149 0.532 0.152 0.958 !       0.63 eA-3
Q150 0.937 0.500 0.234 !       0.63 eA-3
Q151 0.197 0.497 0.297 !       0.62 eA-3
Q152 0.766 0.472 0.486 !       0.62 eA-3
Q153 0.822 0.489 0.578 !       0.61 eA-3
Q154 0.139 0.257 0.706 !       0.61 eA-3
Q155 0.819 0.266 0.407 !       0.60 eA-3
Q156 0.899 0.501 0.828 !       0.60 eA-3
Q157 0.390 0.092 0.171 !       0.60 eA-3
Q158 0.851 0.501 0.937 !       0.60 eA-3
Q159 0.694 0.237 0.733 !       0.60 eA-3
Q160 0.929 0.333 0.017 !       0.60 eA-3
Q161 0.250 0.503 0.984 !       0.59 eA-3
Q162 0.326 0.079 0.233 !       0.59 eA-3
Q163 1.000 0.484-0.002 !       0.59 eA-3
Q164 0.101 0.492 0.469 !       0.59 eA-3
Q165 0.501 0.157 0.923 !       0.59 eA-3
Q166 0.030 0.467 0.124 !       0.59 eA-3
Q167 0.018 0.115 0.812 !       0.59 eA-3
Q168 0.188 0.507 0.000 !       0.58 eA-3
Q169 0.780 0.412 0.472 !       0.58 eA-3
Q170 0.742 0.503 0.062 !       0.58 eA-3
Q171 0.954 0.153 0.250 !       0.58 eA-3
Q172 0.915 0.454 0.716 !       0.58 eA-3
Q173 0.069 0.437 0.236 !       0.58 eA-3
Q174 0.017 0.323 0.174 !       0.58 eA-3
Q175 0.916 0.502 0.406 !       0.57 eA-3
Q176 0.313 0.079 0.257 !       0.57 eA-3
Q177 0.287 0.286 0.289 !       0.57 eA-3
Q178 0.038 0.453 0.176 !       0.57 eA-3
Q179 0.007 0.250 0.879 !       0.57 eA-3
Q180 0.142 0.508 0.891 !       0.57 eA-3
Q181 0.353 0.465 0.186 !       0.57 eA-3
Q182 0.359 0.498 0.812 !       0.56 eA-3
Q183 1.000 0.199 0.078 !       0.56 eA-3
Q184 0.554 0.495 0.109 !       0.56 eA-3
Q185 0.843 0.029 0.310 !       0.56 eA-3
Q186 0.940 0.500 0.281 !       0.56 eA-3
Q187 0.070 0.235 0.238 !       0.56 eA-3
Q188 0.220 0.375 0.295 !       0.56 eA-3
Q189 0.209 0.395 0.097 !       0.55 eA-3
Q190 0.998 0.028 0.203 !       0.55 eA-3
Q191 0.532 0.281 0.894 !       0.55 eA-3
Q192 0.953 0.317 0.842 !       0.55 eA-3
Q193 0.569 0.049 0.750 !       0.55 eA-3
Q194 0.275 0.436 0.485 !       0.55 eA-3
Q195 0.780 0.215 0.346 !       0.55 eA-3
Q196 0.085 0.500 0.812 !       0.55 eA-3
Q197 0.174 0.253 0.668 !       0.55 eA-3
Q198 0.836 0.411 0.519 !       0.55 eA-3
Q199 0.555 0.210 0.238 !       0.55 eA-3
;
_shelxl_version_number           2013-2
_shelx_res_checksum              40668
_shelx_hkl_checksum              49613